{'fraction_non_alphanumeric': 0.03386262924667651, 'fraction_numerical': 0.015029542097488921, 'mean_word_length': 4.774200426439233, 'pattern_counts': {'":': 0, '<': 7, '<?xml version=': 0, '>': 0, 'https://': 0, 'lorem ipsum': 0, 'www.': 0, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 1, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
Solution processed low power organic field-effect transistor bio-chemical sensor of high transconductance efficiency

Developing organic field-effect transistor (OFET) biosensors for customizable detection of biomarkers for many diseases would provide a low-cost and convenient tool for both biological studies and clinical diagnosis. In this work, design principles of the OFET transducer for biosensors were derived to relate the signal-to-noise ratio (SNR) to the device-performance parameters. Steep subthreshold swing (SS), proper threshold voltage (Vth), good-enough bias-stress stability, and mechanical durability are shown to be the key prerequisites for realizing OFET bio-sensors of high transconductance efficiency (gm/ID) for large SNR. Combining a low trap-density channel and a high-k/low-k gate dielectric layer, low-temperature (<100 °C) solution-processed flexible OFETs can meet the performance requirements to maximize the gm/ID. An extended gate-structure OFET biosensor was further implemented for label-free detection of miR-21, achieving a detection limit below 10 pM with high selectivity at a low operation voltage (<1 V).


INTRODUCTION
There are rapidly growing demands for ubiquitous perception of various biomarkers (ions or biomolecules) in blood, body fluids, secretions, excrement, and tissue cells of human for personalized medical diagnosis and healthcare 1,2 . To realize that, the biosensing devices need to be highly customizable to meet diverse system requirements in terms of biocompatibility, cost, and form factor (compact, thin, flexible, or comfortable), while producing output signal of high-enough signal-to-noise ratio (SNR) under strict power constraint. The most affordable and convenient way would be based on electrical measurements, which avoid using additional bulky, power-hungry, and expensive optical components. Transducers made by integration of the sensor interface with a field-effect transistor (FET) have been widely studied, since the FET can convert the sensed signal into an amplified output signal for potentially large SNR 3 . In addition, with FET switches, multiplexed detection in a single reaction is convenient to be implemented for high-throughput and multi-analyte analysis. The organic FET (OFET), composed of organic semiconductors (OSCs) and polymer dielectric layers, shows several competitive advantages over inorganic counterparts for such biosensing applications 4,5 . The use of solution-printing processes and versatile structures might facilitate integration of various sensing interfaces or probes at the device level in great freedom 6 . With low processing temperature and superior intrinsic mechanical flexibility of the full organic stacks, truly flexible sensor electronics can be fabricated using common low Young's modulus thin plastic foils with much less stress-management efforts 7 . In the past, OFETs have been studied for detecting various biomolecules, including enzyme, DNA, and protein [8][9][10][11] . As a popularly used approach, probes are immobilized on the gate or its extended part to capture the target molecules. Once the molecules are being captured, the resulted potential change at the gate is recorded or converted to output-current change through the OFET for further processing. These work well proved that the capability of OFETs to be designed for various biosensing functions through material-and device-structure engineering. However, many of the devices required vacuum processes and inorganic dielectric layers, which would sacrifice the technical competence of the OFET.
Although solution-based processes at low temperature might offer attractive features for high customizability at low cost, they suffer difficulties in fine control of layer thickness, especially for very-thin films, and formation of high-quality semiconductor/dielectric films and interfaces. With such constraints, the achievable device performance is severely limited. In the past, there have been significant efforts on improving the carrier mobility in the OSC channels through material molecule design and crystallizationcontrolled processing methods 12,13 . However, for biochemical sensors to detect very low concentration of analyte in various portable, wearable, or implantable scenarios, large SNR with low operating voltage and power would be a prerequisite [14][15][16] . However, there is lack of studies on optimal design of the OFET for such figure of merits considering the interplay between device structures and material stacks under processing constraints.
This work derives the OFET-design principles for biochemical sensor transducers of large transconductance efficiency (g m /I D ) for large SNR with low operation voltage. Steep subthreshold swing (SS), proper threshold voltage (V th ), and operational stability are shown to be the key parameters to determine the optimal performance. Based on the design principles, low-voltage OFETs are then fabricated on plastic substrate in low-temperature solution processes to obtain the required performance, through formation of a low trap-state density channel interface on high-k/ low-k bilayer-structure gate insulator. To verify its transduction performance, a plastic sensor tag is implemented through encapsulating the OFET with a sensing electrode and a reference electrode for miRNA detection. miRNAs are key biomarkers for many diseases, and label-free miRNA detection in electrochemical ways would provide low-cost and convenient tools for both biological fundamental studies and clinical diagnosis 17 . However, miRNAs are of low charge level due to their short intrinsic molecule length, and thus challenging to be detected at very low concentration. This work demonstrates the feasibility of using the OFET for miRNA sensing. With the optimal device performance, the sensor exhibits a 20% relative output-signal change over the background upon detection of miR-21 (a miRNA biomarker for breast cancer) at 10 pM under an operation voltage less than one volt. Figure 1a illustrates the structure of an OFET-based biochemical sensor, consisting of an OFET transducer with an extended-gate sensing electrode (SE), and a reference electrode (RE). The probeimmobilized SE is to capture analyte targets in solution through specific target/probe combination. For measurement, a constant voltage bias (V Ref ) is applied to the RE, inducing an initial potential at the OFET gate (V GS0 ) through the solution and in turn a channel current in the OFET (I D0 ). As depicted in Fig. 1b, V GS0 can be expressed as:

RESULTS AND DISCUSSION Design principles
where V Chem is the voltage between the RE and the SE, and can be assumed to be a sum of a constant V Chem0 and an interfacial potential drop (V int0 ) 18 . The interfacial potential drop V int0 , arising from the electrode/electrolyte interfacial dipole, is modulated with the captured charged biomolecules and can be measured by using the open circuit potential method 19 . When the SE detects a certain concentration of analyte targets in the solution, the captured negatively (or positively) charged targets would induce a change of the interfacial potential drop (ΔV int ), and thus ΔV GS . Correspondingly, an output-current change (ΔI D ) can be measured by the subsequent readout circuit for digitalization, as shown in Fig. 1a.
The detection limit of the whole system is determined by the signal-to-noise ratio (SNR) of the OFET transducer, which is given as 16,20 SNR ¼ 10 log P signal P noise (2) where P signal is the signal power and P noise is the noise power.
According to the aforementioned analysis, P signal is contributed by ΔI D upon detection of a certain concentration of analyte. For lowfrequency biochemical sensing, P noise is mainly dominated by 1/f noise and can be described as 7 where I is the operation current, K is a process-dependent coefficient, f is the frequency, and α and β are noise parameters (with α = 1 and β = 2 in theory in subthreshold regime). Correspondingly, the SNR for an OFET transducer operating in subthreshold regime at low frequency is deduced to be: According to (4), the SNR depends on the relative currentoutput signal change over the background level (ΔI/I). As a result, to improve the detection limit, it would be important to maximize ΔI D /I D0 of the OFET transducer for a certain concentration of analytes. ΔI D /I D0 can be described as where g m is transconductance and SS is the subthreshold swing. Therefore, to maximize ΔI D /I D0 , enlarging the transconductance efficiency (g m /I D0 ) is as important as achieving effective immobilization of specific targets on the gate electrode (increasing ΔV int ). In other words, g m /I D0 is an important figure-of-merit to benchmark the sensing capability of extended-gate OFET sensors. Since the maximum of g m /I D0 occurs in the subthreshold regime, and is proportional to the inverse of SS 7 , steep SS would thus be required to design OFET transducers of high g m /I D for large SNR.
As illustrated in Fig. 1c, when the OFET is operated in the sensor system, the obtained transfer curve by sweeping V Ref would have a shift compared with the original I D -V GS curve of the OFET. Such a shift is due to the presence of an interfacial potential between the surface of the gate electrode and the aqueous solution 21 . To enable operation of the OFET in the subthreshold regime with a small V Ref , a proper near-zero threshold voltage (V th ) is also required. Operational stability is another concern to be considered, since a certain waiting time (i.e., tens of minutes) is often required for interaction between the probes and the target biomolecules 22 . As illustrated in Fig. 1c, when the OFET is biased in the subthreshold regime, even a slight V th shift would induce significant output-current change (ΔI D ), causing false-positive or false-negative results. Similar to the electrical bias stress, since the flexible device is inevitably subject to some bending state, attention should also be paid to the mechanical durability during bending stress.
According to the above analysis, it is concluded that steep SS, proper threshold voltage, and operational stability under electrical bias and mechanical stress are key prerequisites for designing lowpower OFET biochemical sensor transducers of large SNR.

Target
Probe Subthreshold regime Fig. 1 Illustration of an OFET-based biochemical sensor. a Schematic of the biosensor design for analyte detection in electrolyte solution. The biosensor consists of an OFET transducer and an extended-gate sensing electrode immobilized with probes. V Ref is the bias voltage at the reference electrode (Ag/AgCl). V GS is the resulted gate-to-source voltage on the OFET. I D is the drain current to be measured by the subsequent readout electronic system. b Diagram for potential over a simplified electrochemical cell model with an extended-gate metal as the interfacial material for sensing. The charged molecules captured onto this surface create a potential shift (ΔV int ) at the solution/metal interface and thus equal ΔV GS seen from the OFET. c Illustration of the transfer-curve shift from the I D -V GS curve of the OFET to the I D -V Ref curve when the OFET sensor is tested in solution by sweeping V Ref , and the induced significant output-current change from the background level (ΔI D0 ) in the subthreshold regime even at a small threshold-voltage shift (ΔV th ).

Device fabrication and characterizations
To meet the requirements as discussed above, an OFET design combining a low trap-state density channel and a high-k/low-k gate dielectric layer is implemented, to achieve steep SS and nearzero V th , while using a thick-enough dielectric layer for large-area solution processability. As shown in Fig. 2a, the devices were fabricated in a bottom-gate bottom-contact structure on a polyethylene naphthalate (PEN) plastic substrate. The gate and source/drain electrodes were formed by thermal evaporation of silver (Ag) through shadow masks. The gate dielectric was composed of a low-k poly(vinyl cinnamate) (PVCN) layer and a high-k poly(vinylidene fluoride-trifluoroethylene-chlorofluoroethylene) (P(VDF-TrFE-CFE)) layer with total thickness of about 420 nm, as shown by the cross-sectional scanning electron microscopy (SEM) image (Fig. 2b). Both layers were deposited by spin-coating processes followed by low-temperature annealing. The surfaces of the source/drain electrodes were treated by perfluorobenzenethiol (PFBT) before deposition of the organic semiconductor (OSC) layer. The OSC layer was deposited using a blade-coating process from a blended solution of 6,13-bis (triisopropylsilylethynyl)-pentacene (TIPS-pentacene) and polystyrene (PS) 23 . Well-crystalline structure channels can be formed as shown in Fig. 2c to obtain a low-trap OSC/dielectric interface for steep SS at small-gate dielectric capacitance (20.1 nF·cm −2 ). A CYTOP passivation layer was finally deposited by drop-casting to protect the channel from the air ambient. Details of the fabrication processes are described in "METHODS". The maximum processing temperature is kept below 100°C.
The measured representative transfer (I D -V GS ) and output (I D -V DS ) characteristics of the sealed OFET are shown in Fig. 2d, presenting well-behaved FET behaviors with a steep SS of about 80 mV·dec −1 , a nearly zero V th (0.3 V), and an ON/OFF ratio larger than 10 5 . From the SS value, the effective subgap trap density is estimated to be 4.3 × 10 10 eV −1 ·cm −2 , similar to previous work using a single low-k gate dielectric layer 24 and also superior to those used in extended-gate OFET biosensors (Supplementary Table 1). The measured g m /I D versus V GS is plotted in Fig. 2e, with its maximum value of 28.8 V −1 exceeding those of previously reported extended-gate OFET biosensors (Supplementary Table 1). The maximum g m /I D occurring at V GS = 0.35 V enables the OFET to be used in the sensor system as depicted in Fig. 1a for biomolecule detection of high sensitivity and low detection limit The operational stabilities under continuous switching and constant bias stress were characterized and shown in Fig. 2f. The device exhibits nearly identical transfer characteristics after sweeping between OFF and ON for 120 times. With a bias stress at a V GS near threshold voltage for 3000 s, there is negligible V th shift (less than 0.01 V). The relative current change (ΔI D (t)/I D (0)) is less than 15% after constant bias stress for more than 4 hours. Such a device design owns low-trap OSC/dielectric interface, and is operated with low charge density and weak perpendicular electrical field at low voltage attributed to a thick-gate dielectric layer 25 . Compared with the implemented low-voltage device using ultrathin dielectric of high capacitance, these factors reduce the probability of charge trapping under bias stress, and thus enable the device to achieve high operational stabilities. Large g m / I D , proper V th , and high operational stability make the device a promising transducer for biomolecule detection.

Evaluation of mechanical stability
The mechanical stability of the flexible OFET device encapsulated by CYTOP was evaluated by measuring its electrical characteristics with changing bending angles. Figure 3a  and radius (R) for the OFET under bending test are illustrated in Supplementary Fig. 1. Figure 3b shows the transfer characteristics of the OFET device before and after undergoing bending at various angles, presenting negligible degradation in the subthreshold characteristics even at a large bending angle of about 73˚. The corresponding output characteristics ( Supplementary  Fig. 2) also show no apparent change after bending by about 51˚, while only a slight degradation of on-current was observed after aggressively bending by about 73˚. In this regard, the contact resistance (R C ) during the bending test was further estimated by using a transfer-line method (TLM). It is realized by taking the total normalized on-resistance (R ON ·W) from the output characteristics of OFET devices with various channel lengths in the linear regime and then extrapolating the linear fit to a channel length of zero to obtain R C . As shown in Supplementary Fig. 3, the bent OFETs with channel length ranging from 50 to 110 μm present well-behaved output performance with a clear saturation of the drain current beyond the pinch-off point. Accordingly, the corresponding width-normalized R ON ·W can be calculated and plotted as a function of channel length for OFET under different bending conditions (Supplementary Fig. 4). As shown in Fig. 3c, the R C extracted by TLM at the most significant bending angle of 73˚is approximately 0.3~0.38 MΩ·cm. Although such R C is slightly dependent on the gate bias voltage, it remains nearly unchanged during the measured bending states (Fig. 3d). Electrical measurements of the flexible device were further performed under bending stress. For this purpose, a stressing cycle was applied to the device by repeatedly bending it to radius = 10 mm and immediately releasing it to its initial state at a rate of 12 times per minute. Figure 3e shows that the flexible OFET device maintained well-functional transfer characteristics during the bending stress. Even after 3500 complete cycles, the change in subthreshold swing was not exceeding 5 mV·dec −1 , while threshold voltage shift was less than 0.03 V (Fig. 3f), revealing negligible change in subthreshold performance during the performed bending stress. These results illustrate that the developed low-voltage OFET can sustain the inevitable bending during usage and maintain its electrical performance for proper signal transducing.

Probe immobilization and hybridization
To verify the device concept of the designed OFET transducer for biosensing, this work takes miR-21 detection as an example, which is one of the potential candidate biomarkers for primary breast cancer 26 . The scheme for immobilizing probes on the extendedgate SE is depicted in Fig. 4a. A thiolated single-stranded DNA (ssDNA) probe was designed to match the miR-21 for specific detection. Based on the well-established thiol-gold chemistry, the ssDNA probes and the 6-mercapto-1-hexanol (MCH) were able to self-assemble onto the gold electrode surface efficiently via a strong SH-gold binding. The ssDNA probes work as the receptor for capturing miRNA targets, while the MCH, as a blocking layer, reduces miRNA-gold interaction and thus improves hybridization discrimination 27,28 . As a result, the miR-21 targets were selectively captured on the extended-gate SE through DNA/miRNA hybridization according to the law of Watson-Crick base-pairing 29 .
To verify the hybridization-reaction procedure, miR-21 was labeled with fluorescent dyes (FAM) for fluorescence measurement. As shown in Fig. 4b, the ssDNA-immobilized gold incubated to the 1X phosphate-buffered saline (PBS 1X) solution shows no fluorescence. After incubation of the electrode surface to the FAMlabeled miR-21 solution, there is weak fluorescence at a miR-21 concentration of 10 pM, while obvious fluorescence occurring at a concentration of 1 nM. With increase of the concentration to 100 μM, the signal becomes strong. The results prove the hybridization reaction between the miR-21 targets and the ssDNA probes.

Implementation of miRNA sensor
The individual OFET was cut from the fabricated large area sample, and then encapsulated onto a carrier PEN substrate with the extended-gate SE and the Ag/AgCl RE to complete a sensor tag for use as shown in Fig. 5a. , is shown in Fig. 5d. The solution containing a 3-base mismatch miRNA of a much higher concentration (100 μM) was also tested for comparison. The results show that ΔV th for the lowest measured miR-21 concentration (10 pM) is 16.9 ± 5 mV, much higher than the value (0.2 ± 5 mV) for 3-base mismatch miRNAs of high concentration (100 μM), indicating high selectivity. Moreover, the limit of detection (LOD) was used to interpret the detectability of the sensor. It is defined as the concentration that leads to a sensor response equal to three times the standard deviation of the negative control sample (ΔV th mean ± 3σ), where ΔV th mean is the average response, and σ is the relative standard deviation 30 . According to this definition, the LOD was estimated to be 4.5 pM by taking the response of 3-base mismatch miRNA as the negative control sample. Note that the response at 10 pM is beyond the LOD (Fig. 5d), verifying the OFET biosensor's high sensing capability at such a low concentration. The measured relative current change (ΔI D /I D0 ) at V Ref = −0.1 V for various miR-21 concentrations is shown in Fig. 5e. For a low concentration of 10 pM, ΔI D /I D0 of 20% is able to be obtained for large-enough SNR to be processed by the subsequent readout electronics for digitalization. Therefore, the sensor is able to achieve a detection limit below 10 pM to the target miRNAs with good selectivity at a low operation voltage (<1 V). The overall performance shows competence over that of the previous work based on a Si-FET in Table 1, in terms of the detection limit, the operation voltage, and the static power 31 .
In summary, the derived design principles of the OFET transducer for biosensors build relationships between the SNR and the key OFET-performance parameters, including g m /I D , SS, V th and bias-stress stability. Combining a low trap-state density channel and high-k/low-k structure gate dielectric, OFETs fabricated on PEN substrate with low temperature solution-based processes can meet the optimal design requirements, exhibiting steep SS, near-zero V th , and good-enough bias-stress stability and mechanical durability. Extended-gate structure OFET biosensors were further constructed for label-free detection of miR-21, a potential biomarker for primary breast cancer. The results demonstrate that the sensor can achieve a detection limit below 10 pM to the target miRNAs with good selectivity at a low operation voltage (<1 V). The overall performance is competitive over that of the previous work based on the Si-FET, in terms of the detection limit, the operation voltage and the static power. This work would pave the way to developing low-cost and convenient biosensors based on OFETs to have large SNR for customizable detection of disease biomarkers in both biological studies and clinical diagnosis.

Device fabrication
OFET devices in a bottom-gate bottom-contact structure were fabricated on a plastic PEN foil laminated on a glass carrier. PVCN was dissolved in chlorobenzene with a concentration of 10 mg/ml and spin-coated at 3000 rpm onto the substrate as a planarization layer, followed by UV crosslinking (UV Curer KW-4AC, CHEMAT) for 20 min and then heating at 100°C for 1 h. Next, 40 nm-thick silver (Ag) gate electrodes were deposited by thermal evaporation using a stainless-steel mask. Then, a high-k P (VDF-TrFE-CFE) (dissolved in methyl ethyl ketone, 40 mg/ml) and a low-k PVCN (dissolved in chlorobenzene, 10 mg/ml) were subsequently spincoated to form a thick bilayer-gate dielectric. Ag source/drain (S/D) electrodes were obtained using the same processes as that for formation of the gate electrodes, defining a channel width of 2000 µm and a channel length of 70 µm, respectively. Devices with the same channel width (1500 µm) and a series of channel lengths (50, 70, 90, and 110 µm) were also used to evaluate the mechanical stability. Before the deposition of the semiconductor layer, the sample was immersed into a PFBT solution (5 mM in isopropanol) for 15 min to form self-assembled monolayers on the S/D electrodes. After this treatment, it was carefully rinsed with isopropanol and blown by dry N 2 gas, followed by annealing at 100˚C on a hot plate for 1 min. The semiconductor/polymer-blended solution was prepared by mixing TIPS-pentacene and PS solutions (dissolved in chlorobenzene, 10 mg·mL −1 ) in 3:1 ratio by volume. The semiconducting film was formed using a soft-contact coating approach with a rotatable steel sheet as the meniscus guide at coating speed of 20 mm/s, followed by annealing at 100°C for 30 min 23 . Finally, CYTOP solution (10 µL) was drop-cast to passivate the channel and annealed at 80°C for 30 min.

Sensor-tag encapsulation
After completing the preparation of OFET device, its supporting PEN foil was carefully peeled off from the glass carrier. Subsequently, individual CYTOP-passivated OFET was cut from it to mount onto another holding PEN substrate with prefabricated screen-printed silver interconnects and pads. A bonding process was developed by flipping over the OFET device and attaching to the substrate using silver paste, followed by annealing at 80°C for 10 min. Finally, a silicone sealant was dispensed with a dispenser robot to seal the device.

Sensing-electrode preparation
Extended-gate sensing electrode consisting of chromium (10 nm) and gold (100 nm) was deposited using magnetron sputtering, which was further encapsulated with silicone sealant to define a sensing area of 9 mm 2 . Prior to immobilization of probes, the electrode surface was cleaned by O 2  Transistor Si-FET [31] OFET Detection limit 1 nM <10 pM Operation voltage 1.9 V <1 V Static Power~40 μW < 5 n W ΔI/I 0 at low concentration 37.5% at 1 nM 20% at 10 pM plasma for 10 min. Then, 10 μL of 5′-SH-modified capture ssDNA solution (10 -4 M, dissolved in PBS 1X) was added onto the gold electrode and incubated at 4°C in humid condition overnight, followed by rinsing thoroughly with PBS 1X solution. After immobilization of probes, the electrode was posttreated with 10 μL of MCH aqueous solution (1 mM) for 1 h to remove nonspecifically bound oligonucleotides and block extraactive gold surface, followed by rising with PBS 1X solution. The obtained sensing electrodes were used immediately to subject to 10 μL of fully complementary targets (miR-21 or FAM-dyed miR-21) and noncomplementary targets (3-base mismatch miRNA) diluted to desired concentrations in PBS 1X solutions for hybridization, respectively, followed by rinsing with PBS 1X solution carefully.

Characterization and measurement
The polarized optical micrograph for TIPS-pentacene crystalline was taken with a microscope (XPF-300C, Caikon). The fluorescence images were obtained from inverted fluorescence microscopy (IX71, Olympus Life Science). The cross-sectional scanning electron microscopy (SEM) image was obtained on a Zeiss Ultra Plus Field Emission Scanning Electron Microscope at an electric voltage of 5 kV. The cyclic bending test of the flexible OFET was performed on a stretching machine at bending radius of 10 mm with a speed of 5 s/cycle. The sensor tag was connected to the extended-gate sensing electrodes and reference electrode (Ag/AgCl) via copper wires. The electrical characterizations of the OFETs and biosensors were performed using a semiconductor parameter analyzer (Keithley 4200 system). All measurements were carried out at room temperature in ambient air.